20 TRANSPORTATION RESEARCH RECORD 1217
Effect of Compaction on Asphalt Concrete Performance
ROBERT N. LINDEN, }OE P. MAHONEY, AND NEWTON c. JACKSON
This paper presents information on how compnction (specifi-cally, air voids) influences the performance of dense asphalt concrete pavement surfaces. The information is based on three separate sources: the exiting literature on the subject, a ques-tionnaire survey or 48 state highway agencies on compaction practice, and per for mance data from the Washington State Pavement Management System. All three information sources show some correlation between the degree or compaction and the performance of asphalt concrete pavement. Overall, a 1 percent increase in air voids (over the base air-void level of 7 percent) tends to produce about a 10 percent loss in pavement life.
This paper is the result of research on how compaction-specifically, air voids-affects the performance of dense asphalt concrete pavement. Three information sources support the findings: a literature review; a survey of state highway agen-cies (SHAs); and data from the Washington State Pavement Management System (WSPMS).
Other researchers have found that asphalt concrete perfor-mance is in part a function of compaction, and hence air voids, in dense mixtures . Two frequently used terms indicative of performance are fatigue cracking and aging.
Fatigue cracking (or "alligator cracking") usually describes cracked pavement that has been repeatedly bent by heavy traffic. Researchers might reasonably ask how air voids affect asphalt concrete fuLiguc life.
Several authors (J- 3) have shown that the fatigue life (time from original construction to substantial fatigue cracking) of asphalt concrete is reduced from 10 to 30 percent for each 1 percent increase over normal in air voids. For example, if 7 percent air voids are achievable for a mix yet 11 percent air voids resulted from construction, one could expect about a 40 percent reduction in pavement surfacing life (11 percent minus 7 percent equals 4, times 10 percent).
R . N. Linden , Consulting Engineer, 51 W. Dayton , Edmonds, Wash. 98020. J.P. Mahoney, Department of Civil Engineering, University of Washington, Seattle, Wash. 98195. N. C. Jackson , Washington State Department of Transportation , Olympia , Wash. 98504 .
Another way to approach air voids is to ask how they affect the thickness of asphalt concrete . As demonstrated by Finn and Epps (J), the effective thickness of asphalt concrete layers decreases as air voids increase . Finn and Epps evaluated two thicknesses of asphalt concrete, 4 and 6 in. , at a starting point of 7 percent air voids (7 percent is generally considered achiev-able in normal paving construction) . The following tabulation summarizes their findings.
Percent Air Voids in A sphalt Concrete
7 8 9
. 10 12
Effective Thickness of Asphalt Concrete (in .)
4.0 3.5 3.0 2.5 2.0
6.0 5.0 4.5 4.0 4.0
Thus, if the air voids are increased from a desirable level of 7 percent to a very poor compaction level of 12 percent, a 4-in.-thick asphalt concrete layer effectively lasts only as long as a 2-in. layer; a 6-in. layer is reduced to the effectiveness of a 4-in.-thick layer.
Aging of asphalt concrete can be evaluated in many ways. One way pertinent to this research is to judge aging by con-sidering asphalt penetration and determining how air voids affect that property.
Goode and Owings ( 4) showed that, for asphalt concrete mixtures 4 years after construction , asphalt penetration is reduced about 6 percent for each 1 percent increase in air voids. They demonstrated, for example , that mixes retain about 75 percent of their original (immediately after construc-tion) asphalt penetration at an air void level of 6 percent. If the air voids immediately after construction are 12 percent, however, the asphalt penetration is only 30 percent of its original level. The lower the asphalt penetration, the more susceptible the mixture is to cracking, as established by Hub-bard and Gollomb (5), who showed that asphalt penetration of 30 or less (at 77F) generally leads to distressed asphalt concrete . High-air-void pavements, as Goode and Owings ( 4) conclude , can be expected to result in low penetration levels for asphalt cement whose penetration level before mixing was at 85-100.
Linden et al.
Air Void Levels
The work of the authors discussed above corroborates the findings of Finn et al. (6) concerning the maximum air void levels desirable for asphalt concrete construction. Those levels are summarized below.
Asphalt Concrete Layer
Upper 1 Yi--2 in. of asphalt concrete pavement Asphalt concre te pave-ment deeper than 2 in.
Maximum Air Voids (%)
Moderate to Heavy Traffic
Results of the SHA survey also support the levels estab-lished by Finn et al.
A questionnaire (7) was prepared and sent in 1987 to the materials engineer in each of the 50 SHAs. The question-naire's purpose was to review practice and gather opinions of the SHAs on the control of air voids in asphalt concrete pave-ments. Each agency was asked to respond to eight questions on methods of mix design, construction compaction control and tests, field density limits and average asphalt content, pavement air voids, primary mode of pavement failure, and, finally, the effect of increasing air voids on pavement life. Forty-eight agencies responded to the questionnaire .
It should be noted that some questions are subjective; answers may be based on the respondent's opinion rather than on data.
A sample completed questionnaire is shown in Figure 1. Each question and a summary of agency responses follow. (Percentage figures for number of agencies responding have been rounded to the nearest whole percentage point.)
1. Asphalt concrete mix design procedure (a) Marshall method (b) Hveem method (c) Other (please specify)
Responses are summarized in the following table . Two agen-cies use both Marshall and Hveem methods . Other methods used are aggregate gradation and AASHTO T-167 .
No. of A gencies Percent of 48 Method Using Method Respondents
Marshall 34 71 Hveem 10 21 Both 2 4 Other 2 4
2. Are field results used to verify the adequacy of asphalt concrete mix designs? Yes __ No __ . If yes, what types of field data are considered?
Yes-39 agencies (81 percent) No-9 agencies (19 percent) Agencies that responded yes typically use field results to
verify air voids, aggregate gradation , asphalt content, and so on.
3. Construction compaction requirement (i) Percent of laboratory-compacted density
(ii) Percent of theoretical maximum density (i.e., zero air voids)
(iii) Percent of control strip density (e .g., target = 95 % of control strip)
(iv) Other (please specify)
(i) Percent of laboratory compacted density-18 agen-cies (38 percent)
(ii) Percent of theore tical maximum den ity (TMD) (AASHTO 1'209-82)- 21 agencies (44 percent)
(iii) Percent of control strip density-6 agencie (12 percent)
(iv) Other-3 agencies (6 percent), which reported per-cent of field Marshall density
4. Construction compaction control tests (a) Nuclear densimeter (b) Core samples (c) Other (please specify)
Eighteen agencies indicated use of both nuclear gauge and core samples. The core samples are most likely used to cal-ibrate the nuclear gauge when both methods are specified.
(a) Nuclear gauge - 18 agencies (38 percent) (b) Core samples - 12 agencies (25 percent) (c) Other - 18 agencies (38 percent), which reported
using both methods
QUESTIONNAIRE ON EFFECT OF AIR VOIDS ON ASPHALT CONCRETE PERFORMANCE
Please answer the following questions with respect to your agency's procedures or requirements for construction control of a sphalt concrete pavement . In this questionnaire air voids are defined as the air spaces that occur between the coated aggregate particles in the final compacted asphalt concrete mixture.
l. Asphalt concrete mix desfgn procedure (a) Marshall method (b) Hveem method x (c) Other (pleas_e_s_p-ec-1~f~y~).-------~~--~--------
2. Are field results used to ver1fy the adequacy of asphalt
concrete mix designs? Yes x No If yes, what types of field data are cons1dered7
Construction compaction requirement (i) Percent of laboratory compacted density (ii) Percent of theoretical maxi~um density __ __;x;.:_ ____ _
(1.e., zero air voids) (ii1) Percent of control strip density
(e.g. target 95% of control strip) (1v) Other (please specify) X-Roller passes for peak dens ity Compaction spec1f1cations - Please 1nclude a copy of ( no~ .mafn your standard specification for asphalt concrete ine compaction with the questionnaire.
4. Construction compaction control tests (a) Nuclear densimeter ___ _ ~x~------------------(b) Core suples (c) Other (pleas-e--sp_e_c_f_f_y~)------------
5. Construction compaction control criteria (a) Does the Agency have 1 Maximum field density liit?
Yu No x If yes, what is the limit (percent) I
(b) What do you normally do 1f 1 contr&ctor exceeds your axi~um compaction requtre~ents7
Does the Agency have a mfnfmum ffeld density 11m1t7 Yes X No ____ ___ If yes, what 1s the l1mft7 (percent} 92 S of Rice What do you nor~ally do if a contractor does not eet Density your mfnimum compaction requirements?